Download presentation

Presentation is loading. Please wait.

Published bySterling Want Modified about 1 year ago

1
Stereology applied to GBCD Texture, Microstructure & Anisotropy A.D. Rollett Last revised: 19 th Mar. ‘14 1

2
Objectives To instruct in methods of measuring characteristics of microstructure: grain size, shape, orientation; phase structure; grain boundary length, curvature etc. To describe methods of obtaining 3D information from 2D cross-sections: stereology. To show how to obtain useful microstructural quantities from plane sections through microstructures. In particular, to show how to apply stereology to the problem of measuring 5-parameter Grain Boundary Character Distributions (GBCD) without having to perform serial sectioning. Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions 2

3
Stereology: References These slides are partly based on: Quantitative Stereology, E.E. Underwood, Addison-Wesley, equation numbers given where appropriate. Also useful: M.G. Kendall & P.A.P. Moran, Geometrical Probability, Griffin (1963). Kim C S and Rohrer G S Geometric and crystallographic characterization of WC surfaces and grain boundaries in WC-Co composites. Interface Science, (2004). C.-S. Kim, Y. Hu, G.S. Rohrer, V. Randle, "Five-Parameter Grain Boundary Distribution in Grain Boundary Engineered Brass," Scripta Materialia, 52 (2005) Miller HM, Saylor DM, Dasher BSE, Rollett AD, Rohrer GS. Crystallographic Distribution of Internal Interfaces in Spinel Polycrystals. Materials Science Forum :783 (2004). Rohrer GS, Saylor DM, El Dasher B, Adams BL, Rollett AD, Wynblatt P. The distribution of internal interfaces in polycrystals. Z. Metall. 2004; 95:197. Saylor DM, El Dasher B, Pang Y, Miller HM, Wynblatt P, Rollett AD, Rohrer GS. Habits of grains in dense polycrystalline solids. Journal of The American Ceramic Society 2004; 87:724. Saylor DM, El Dasher BS, Rollett AD, Rohrer GS. Distribution of grain boundaries in aluminum as a function of five macroscopic parameters. Acta mater. 2004; 52:3649. Saylor DM, El-Dasher BS, Adams BL, Rohrer GS. Measuring the Five Parameter Grain Boundary Distribution From Observations of Planar Sections. Metall. Mater. Trans. 2004; 35A:1981. Saylor DM, Morawiec A, Rohrer GS. Distribution and Energies of Grain Boundaries as a Function of Five Degrees of Freedom. Journal of The American Ceramic Society 2002; 85:3081. Saylor DM, Morawiec A, Rohrer GS. Distribution of Grain Boundaries in Magnesia as a Function of Five Macroscopic Parameters. Acta mater. 2003; 51:3663. Saylor DM, Rohrer GS. Determining Crystal Habits from Observations of Planar Sections. Journal of The American Ceramic Society 2002; 85:2799. Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions 3

4
Questions 1.What is the connection between lines/traces observed on planar cross-sections of 3D interfaces and surface area? 2.How does Buffon’s Needle measure π? 3.What is the definition of Stereology? 4.What are some examples of measureable quantities and derived quantities in stereology? 5.What is an accumulator diagram/stereogram? 6.When we observe the trace of a boundary/interface in a cross- section, what can we infer about the true normal to that interface? 7.How do we use the trace, once converted to crystal coordinates, in an accumulator stereogram? What is the standard discretization of the (hemi- )spherical accumulator stereogram? Why do we divide up the declination (co-latitude) angle in increments of cos( )? What is the key difference between analyzing surface normals and grain boundaries (to get the GBCD)? Given a 3D microstructure (i.e. image as an orientation map), what is the best way to proceed to extract grain boundary normals (and misorientations)? What units do we (typically) use for GBCD and Misorientation Distributions? 4

5
5 Measurable Quantities N := number (e.g. of points, intersections) P := points L := line length Blue easily measured directly from images A := area S := surface or interface area V := volume Red not easily measured directly Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions

6
6Definitions Subscripts: P := per test point L := per unit of line A := per unit area V := per unit volume T := total overbar:= average = average of x E.g. P A := Points per unit area Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions [Underwood]

7
Relationships between Quantities V V = A A = L L = P P mm 0 S V = (4/π)L A = 2P L mm -1 L V = 2P A mm -2 P V = 0.5L V S V = 2P A P L mm -3 (2.1-4). These are exact relationships, provided that measurements are made with statistical uniformity (randomly). Obviously experimental data is subject to error. Notation and Eq. numbers from Underwood, 1971 Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions 7

8
Measured vs. Derived Quantities Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions Remember that it is not easy to obtain true 3D measurements (squares) and so we must find stereological methods to estimate the 3D quantities (squares) from 2D measurements (circles). 8 Relationships between Quantities

9
Surface Area (per unit volume) S V = 2P L (2.2). Derivation based on random intersection of lines with (internal) surfaces. Probability of intersection depends on inclination angle, . Averaging gives factor of 2. Clearly, the area of grain boundary per unit volume is measured by S V. Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions 9

10
S V = 2P L Derivation based on uniform distribution of elementary areas. Consider the dA to be distributed over the surface of a sphere. The sphere represents the effect of randomly (uniformly) distributed surfaces. Projected area = dA cos . Probability that a vertical line will intersect with a given patch of area on the sphere is proportional to projected area of that patch onto the horizontal plane. Therefore we integrate both the projected area and the total area of the hemisphere, and take the ratio of the two quantities Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions 10

11
S V = 2P L Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions 11

12
12 Length of Line per Unit Area, L A versus Intersection Points Density, P L Set up the problem with a set of test lines (vertical, arbitrarily) and a line to be sampled. The sample line can lie at any angle: what will we measure? ref: p38/39 in Underwood This was first considered by Buffon, Essai d’arithmetique morale, Supplément à l’Histoire Naturelle, 4, (1777) and the method has been used to estimate the value of π. Consequently, this procedure is also known as Buffon’s Needle. Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions

13
13 L A = π/2 P L, contd. The number of points of intersection with the test grid depends on the angle between the sample line and the grid. Larger value means more intersections. The projected length = l sin = l P L ∆x. Line length in area, L A ; consider an arbitrary area of x by x : l sin l cos l ∆x, or d Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions Therefore to find the relationship between P L and L A for the general case where we do not know ∆x, we must average over all values of the angle

14
14 L A = π/2 P L, contd. Probability of intersection with test line given by average over all values of : Density of intersection points, P L, to Line Density per unit area, L A, is given by this probability. Note that a simple experiment estimates π (but beware of errors!). Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions

15
15 Buffon’s Needle Experiment In fact, to perform an actual experiment by dropping a needle onto paper requires care. One must always perform a very large number of trials in order to obtain an accurate value. The best approach is to use ruled paper with parallel lines at a spacing, d, and a needle of length, l, less than (or equal to) the line spacing, l ≤ d. Then one may use the following formula. (A more complicated formula is needed for long needles.) The total number of dropped needles is N and the number that cross (intersect with) a line is n. Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions See: Also

16
S V = (4/π)L A If we can measure the line length per unit area, L A, directly, then there is an equivalent relationship to the surface area per unit volume, S V. This relationship is immediately obtained from the previous equation and a further derivation (not given here) known as Buffon’s Needle: S V / 2 = P L and P L = (2/π) L A, which together give: S V = (4/π) L A. Careful! This simple analysis leads to an elegant experiment which consists of dropping a needle on ruled paper and counting intersections. This is, however, an inefficient way of estimating π. In the OIM software, for example, grain boundaries can be automatically recognized based on misorientation and their lengths counted to give an estimate of L A. From this, the grain boundary area per unit volume can be estimated (as S V ). Objectives Notation Equations Delesse S V -P L L A -P L Topology Grain_Size Distributions 16

17
Example Problem: Tungsten Carbide Example Problem (Changsoo Kim, Prof. G. Rohrer): consider a composite structure (WC in Co) that contains faceted particles. The particles are not joined together although they may touch at certain points. You would like to know how much interfacial area per unit volume the particles have (from which you can obtain the area per particle). Given data on the line length per unit area in sections, you can immediately obtain the surface area per unit volume, provided that the sections intersect the facets randomly. 17

18
Faceted particles, contd. An interesting extension of this problem is as follows. What if each facet belongs to one of a set of crystallographic facet types, and we would like to know how much area each facet type has? What can we measure, assuming that we have EBSD/OIM maps? In addition to the line lengths of grain boundary, we can also measure the orientation of each line. If the facets are limited to a all number of types, say {100}, {111} and {110}, then it is possible to assign each line to one type (except for a few ambiguous positions). This is true because the grain boundary “line” that you see in a micrograph must be a tangent to the boundary plane, which means that it must be perpendicular to the boundary normal. In crystallographic terms, it must lie in the zone of the plane normal. 18

19
Determining Average 3-D Shape for WC Problem : Crystals are three-dimensional, micrographs are two-dimensional Do these WC crystals have a common, crystallographic shape? 60 x 60 m 2 Serial sectioning : - labor intensive, time consuming - involves inaccuracies in measuring each slice especially in hard materials 3DXDM : - needs specific equipment, i.e. a synchrotron! 19

20
We know that each habit plane is in the zone of the observed surface trace Assumption : Fully faceted isolated crystalline inclusions dispersed in a second phase For every line segment observed, there is a set of possible planes that contains a correct habit plane together with a set of incorrect planes that are sampled randomly. Therefore, after many sets of planes are observed and transformed into the crystal reference frame, the frequency with which the true habit planes are observed will greatly exceed the frequency with which non-habit planes are observed. Measurement from Two-Dimensional Sections [Changsoo Kim, 2004] 20 Notation: l ij : trace of j th facet of the i th particle n ijk : normal, perpendicular to trace.

21
Transform Observations to Crystal Frame Transformation (orientation) matrix from (Bunge) Euler angles: c : cosine, s : sine Vector components in crystal reference frame Vector components in laboratory reference frame 100x100 m 2 [Changsoo Kim, 2004] 21

22
Therefore, if we repeat this procedure for many WC grains, high intensities (peaks) will occur at the positions of the habit plane normals X X X X X X [Changsoo Kim, 2004] Trace Pole Poles of possible planes Observed surface trace transform to crystal reference frame 22 Basic Idea Draw the zone of the Trace Pole: The normal to a given facet type is always perpendicular to its trace:

23
Crystallography Step 1: identify a reference direction. Step 2: identify a tangent to a grain boundary for a specified segment length of boundary. Step 3: measure the angle between the g.b. tangent and the reference direction. Step 4: convert the direction, t sample, in sample coordinates to a direction, t crystal, in crystal coordinates, using the crystal orientation, g. Steps 2-4: repeat for all boundaries Step 5: classify/sort each boundary segment according to the type of grain boundary. t crystal = g t sample t sample WC in Co, courtesy of Changsoo Kim 23

24
Faceted particles, facet analysis Red poles must lie on {110} facets Blue poles must lie on {100} facets Discussion: where would you expect to find poles for lines associated with {111} facets? The set of measured tangents, {t crystal } can be plotted on a stereographic projection 24

25
Faceted particles, area analysis The results depicted in the previous slide suggest (assuming equal line lengths for each sample) that the ratio of values is: L A/110 : L A/100 = 6:4 S V/110 : S V/100 = 6:4 From these results, it is possible to deduce ratios of interfacial energies. 25

26
The probability that a plane is observed is proportional to sin k and to the line length |l ij |. Planes parallel to the section plane are not observed whereas planes perpendicular to the section have the maximum probability of being observed. When this probability is plotted as a function of the normal, n’, (in the crystal frame) maxima will occur at the habit planes. Habit Probability Function The dot product of any l ij with each habit plane vanishes for the habit plane that created the surface trace. Since the total length of a set of randomly distributed lines intersecting an area is proportional to that area, the ratios of the line lengths associated with each plane is an estimate of the relative surface areas. 3D reconstruction : [Changsoo Kim, 2004] 26

27
½ of the total grid Numerical Analysis Discretization Grid discretization in increments of and (cos ) gives equal area for each cell Probability function, normalized to give units of: Multiples of Random Distribution (MRD) [Changsoo Kim, 2004] 27 Procedure: compute a series of points along the zone of each trace pole and bin them in the crystal frame.

28
15 grains ++ …. = 30 grains50 grains200 grains 1 line segment of 1 grain 2 line segments of 1 grain another line segment of 1 grain + = another grain [Changsoo Kim, 2004] 28

29
Results (0001) ~50 WC grains~200 WC grains (0001) There are two habit planes, basal plane (0001) and prism plane High MRD values occur at the same positions of 50 and 200 WC grain tracings Only 200 grains are needed to determine habit planes because of the small number of facets [Changsoo Kim, 2004] 29

30
Five parameter grain boundary character distribution (GBCD) Three parameters for the misorientation : g i,i+1 j r ij1 r ij2 n’ ij l’ ij Two parameters for the orientation: n ij Grain boundary character distribution: ( g, n), a normalized area measured in MRD 30

31
Direct Measurement of the Five Parameters n n n Record high resolution EBSP maps on two adjacent layers. Assume triangular planes connect boundary segments on the two layers. ∆g and n can be specified for each triangular segment Saylor, Morawiec, Rohrer, Acta Mater. 51 (2003)

32
Stereology for Measuring g and n The probability that the correct plane is in the zone is 1. The probability that all planes are sampled is < 1. Trace pole Poles of possible planes The grain boundary surface trace is the zone axis of the possible boundary planes. transform to the misorientation reference frame gg D.M. Saylor, B.L. Adams, and G.S. Rohrer, "Measuring the Five Parameter Grain Boundary Distribution From Observations of Planar Sections," Metallurgical and Materials Transactions, 35A (2004) NB each trace contributes two poles, zones, one for each side of the boundary 32

33
Illustration of Boundary Stereology Grain boundary traces in sample reference frame All planes in the zone of trace, in the misorientation frame (at a fixed g) The background of accumulated false signals must then be subtracted. The result is a representation of the true distribution of grain boundary planes at each misorientation. A continuous distribution requires roughly 2000 traces for each g 33

34
Background Subtraction Each tangent accumulated contributes intensity both to correct cells (with maxima) and to incorrect cells. The closer that two cells are to each other, the higher the probability of “leakage” of intensity. Therefore the calculation of the correction is based on this. The correct line length in the i th cell is l i c and the observed line length is l i o. The discretization is specified by D cells over the angular range of the accumulator (stereogram). 34

35
Background Subtraction: detail X X X X X X Recall the basic approach for the accumulator diagram: Take the “correct” location of intensity at 111; the density of arcs decreases steadily as one moves away from this location. This is the basis for the non-uniform background correction. 35

36
Background Subtraction: detail The basis for the correction given by Saylor et al. is simplified to two parts. 1.A correction is applied for the background in all cells. 2.A second correction is applied for the nearest neighbor cells to each cell. In more detail: 1.The first correction uses the average of the intensities in all the cells except the one of interest, and the set of nearest neighbor (NN) cells. 2.The second correction uses the average of the intensities in just the NN cells, because these levels are higher than those of the far cells. Despite the rather approximate nature of this correction, it appears to function quite well. 36

37
Background Subtraction: detail The correction given by Saylor et al. is based on fractions of each line that do not belong to the point of interest. Out of D cells along each line (zone of a trace) D-1 out of D cells are background. The first order correction is therefore to subtract (D-1)/D multiplied by the average intensity, from the intensity in the cell of interest (the i th cell). This is then further corrected for the higher background in the NN cells by removing a fraction Z (=2/D) of this amount and replacing it with a larger quantity, Z(D-1) multiplied by the intensity in the cell of interest ( l i c ). 37

38
Texture effects, limitations If the (orientation) texture of the material is too strong, the method as described will not work. Texture effects can be mitigated by taking sections with different normals, e.g. slices perpendicular to the RD, TD, ND. No theory is available for how to quantify this issue (e.g. how many sections are required?). 38

39
Examples of 2-Parameter GBCD Important limitation of the stereological approach: it assumes that the (orientation) texture of the material is negligible. The next several slides show examples of 2-parameter and 5- parameter distributions from various materials. The 2-parameter distributions are equivalent to posing the question “how does the boundary population vary with plane/normal, regardless of misorientation?” Intensities are given in terms of multiples of a random (uniform) intensity (MRD/MUD). Grain boundary populations are computed for only the boundary normal (and the misorientation is “averaged out”). These can be compared with surface energies. 39

40
Examples of Two Parameter Distributions Grain Boundary Population ( g averaged) MgO SrTiO 3 Sano et al., J. Amer. Ceram. Soc., 86 (2003) Measured Surface Energies Saylor & Rohrer, Inter. Sci. 9 (2001)

41
Examples of Two Parameter Distributions MgAl 2 O 4 Grain Boundary Population ( g averaged) Surface Energies/habit planes TiO 2 Ramamoorthy et al., Phys. Rev. B 49 (1994)

42
Examples of Two Parameter Distributions < Al 2 O 3 Grain Boundary Population ( g averaged) Surface Energies/habits WC Kitayama and Glaeser, JACerS, 85 (2002)

43
Examples of Two Parameter Distributions Fe-Si Gale et al. Phil. Mag. 25 (1972) >1.0 Al Grain Boundary Population ( g averaged) Measured Surface Energies Nelson et al. Phil. Mag. 11 (1965) Saylor et al. (2004) Acta mater Bennett et al. (2004) Recrystallization and Grain Growth, :

44
Examples of 5-parameter GBCDs Next, we consider how the population varies when the misorientation is taken into account Each stereogram corresponds to an individual misorientation: as a consequence, the crystal symmetry is (in general) absent because the misorientation axis is located in a particular asymmetric zone in the stereogram. It is interesting to compare the populations to those that would be predicted by the CSL approach. Note that the pure twist boundary is represented by normals parallel to (coincident with) the misorientation axis. Pure tilt boundaries lie on the zone of the misorientation axis. The misorientation axis is always placed in the triangle. 44

45
(a) (b) (c) (d) 40° 9 MRD 38°= 7 60°= 3 Grain Boundary Distribution in Al: [111] axes ( g, n) (n) (n|40°/[110]) (n|38°/[111]) (n|60°/[111]) (111) Twist boundaries are the dominant feature in (∆g,n) (221) (114) tilt boundaries analyzed in an Al thin film, annealed at 400°C. 77 45 Misorientation axis always in this SST

46
(n) for low CSL misorientations: SrTiO 3 MRD 33 55 77 99 Except for the coherent twin, high lattice coincidence and high planar coincidence do not explain the variations in the grain boundary population. (211) (031) (012) (321) (221) (114) 46

47
Distribution of planes at a single misorientation Twin in TiO 2 66° around [100] or, 180° around [100] (011) (n|66°[100]) 47

48
0)2(11 0)1(10 (0001) MRD Plane orientations for grain boundaries with a 30 misorientation about [0001] Plane orientations for grain boundaries with a 90 misorientation about 0)1(10 MRD Distribution of planes at a single misorientations: WC 48

49
Ni -brass Cubic close packed metals with low stacking fault energies Preference for the (111) plane is stronger than in Al, but this is mainly a consequence of the high frequency of annealing twins in low to medium stacking-fault energy fcc metals. MRD (n) 49

50
Grain Boundary Engineered -Brass 9 3.8% of total area planes at 9: (n|39°/[110]) 9 2.8% of total area MRD all planes, (n) Strain-recrystallization cycle 1 Strain-recrystallization cycle 5 MRD [110] Influence of GBCD on Properties: Experiment The engineering of the GBCD leads to a 40% increase in ductility: V. Randle, Phil. Mag. A (2001) MRD Difference (SR5-SR1) 14 The increase in ductility can be linked to increased dislocation transmission at grain boundaries. 50

51
MRD (n), averaged over all misorientations ( g) Effect of GB Engineering on GBCD Al MRD MRD all boundaries twins removed With the exception of the twins, GBE brass is similar to Al Can processes that are not permitted to reach steady state be predicted from steady state behavior (grain boundary engineering)? -brass 51

52
Ca-doped MgO, grain size: 24 m MRD Undoped MgO, grain size: 24 m Larger GB frequency range of Ca-doped MgO suggests a larger GB energy anisotropy than for undoped MgO Experiment: compare the GBCD and GBED for pure (undoped) and doped materials 75 52

53
Δγ = 1.09 Δγ = 0.46 Ca solute increases the range of the gb / s ratio. The variation of the relative energy in undoped MgO is lower (narrower distribution) than in the case of doped material. Grain Boundary Energy Distribution is Affected by Composition 1 m 76 53

54
Range of GB / S (on log scale) is smaller for Bi-doped Ni than for pure Ni, indicating smaller anisotropy of GB / S. This correlates with the plane distribution Bi impurities in Ni have the opposite effect Pure Ni, grain size: 20 m Bi-doped Ni, grain size: 21 m 77 54

55
Conclusions Statistical stereology can be used to reconstruct a most probable distribution of boundary normals, based on their traces on a single section plane. Thus, the full 5-parameter Grain Boundary Character Distribution can be obtained stereologically from plane sections, provided that the texture is weak. The tendency for grain boundaries to terminate on planes of low index and low energy is widespread in materials with a variety of symmetries and cohesive forces. The observations reduce the apparent complexity of interfacial networks and suggest that the mechanisms of solid state grain growth may be analogous to conventional crystal growth. 55

56
Questions What is an accumulator diagram? Why do we transform grain boundary traces from the sample frame to the crystal frame? What is stereology? Which quantities can be measured directly from cross-sections? What is the stereological relationship between line length (e.g. of grain boundaries) measured in cross-section to surface area per unit volume? How does frequency of grain boundary type relate to surface energy? 56

57
Questions - 2 What is the significance, if any of the CSL concept in terms of grain boundary populations? Which CSL types are actually observed in large numbers (and in which materials)? How does grain boundary frequency relate to grain boundary energy? What is “Buffon’s Needle”? How does stereology help us to measure the Grain Boundary Character Distribution? What are typical 1-, 3-, 5- and 2-parameter plots of GB character? 57

58
Supplemental Slides Details about how to construct the zone to an individual pole in a stereogram that represents a (hemi-)spherical space. Details about how texture affects the stereological approach to determining GBCD. 58

59
Boundary Tangents A more detailed approach is as follows. Measure the (local) boundary tangent: the normal must lie in its zone. A B n s (A) x1x1 t s (A) x2x2 gAgA gBgB 59

60
G.B. tangent: disorientation Select the pair of symmetry operators that identifies the disorientation, i.e. minimum angle and the axis in the SST. 60

61
Tangent Boundary space Next we apply the same symmetry operator to the tangent so that we can plot it on the same axes as the disorientation axis. We transform the zone of the tangent into a great circle. Boundary planes lie on zone of the boundary tangent: in this example the tangent happens to be coincident with the disorientation axis. Disorientation axis 61

62
Tangent Zone The tangent transforms thus: t A = O A g A t S (A) This puts the tangent into the boundary plane (A) space. To be able to plot the great circle that represent its great circle, consider spherical angles for the tangent, { t, t }, and for the zone (on which the normal must lie), { n, n }. 62

63
Spherical angles “chi” := declination “phi” := azimuth Pole of tangent has coordinates ( t, t ) Zone of tangent ( n, n ) 63

64
Tangent Zone, parameterized The scalar product of the (unit) vectors representing the tangent and its zone must be zero: To use this formula, choose an azimuth angle, t, and calculate the declination angle, n, that goes with it. 64

65
Effect of Texture: Distribution of misorientation axes in the sample frame To make a start on the issue of how texture affects stereological measurement of GBCD, consider the distribution of misorientation axes. In a uniformly textured material, the misorientation axes are also uniformly (randomly) distributed in sample space. In a strongly textured material, this is no longer true, and this perturbs the stereology of the GBCD measurement. For example, for a strong fiber texture, e.g. //ND, the misorientation axes are also parallel to the common axis. Therefore the misorientation axes are also //ND. This means that, although all types of tilt and twist boundaries may be present in the material (for an equi-axed grain morphology), all the grain boundaries that one can sample with a section perpendicular to the ND will be much more likely to be tilt boundaries than twist boundaries. This then biases the sampling of the boundaries. In effect, the only boundaries that can be detected are those along the zone of the 111 pole that represents the misorientation axis (see diagram on the right). Misorientation axis, e.g

66
GBCD in annealed Ni This Ni sample had a high density of annealing twins, hence an enormous peak for 111/60° twist boundaries (the coherent twin). Two different contour sets shown, with lower values on the left, and higher on the right, because of the variation in frequency of different misorientations. 66

67
Misorientation axes: Ni example Now we show the distributions of misorientation axes in sample axes, again with lower contour values on the left. Note that for the 111/60° case, the result resembles a pole figure, which of course it is (of selected 111 poles, in this case). The distributions for the 111/60° and the 110/60° cases are surprisingly non-uniform. However, no strong concentration of the misorientation axes exists in a single sample direction. 67

68
Zones of specimen normals in crystal axes (at each boundary) An alternate approach is to consider where the specimen normal lies with respect to the crystal axes, at each grain boundary (and on both sides of the boundary). Rather than drawing/plotting the normal itself, it is better to draw the zone of the normal because this will give information on how uniformly, or otherwise, we are sampling different types of boundaries. Note that the crystal frame is chosen so as to fix the misorientation axis in a particular location, just as for the grain boundary character distributions. ∆g nAnA nBnB Zone of A Zone of B 68

69
Zones of specimen normals: Ni example Again, two different scales to add visualization with lower values on the left. Note that the 111 cases are all quite flat (uniform). The 110/60° case, however, is far from flat, and two of the 3 peaks coincide with the peaks in the GBCD. 69

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google